Presentation on theme: "Chapter 9 Thin film deposition"— Presentation transcript:
1 Chapter 9 Thin film deposition Introduction to thin film deposition.Introduction to chemical vapor deposition (CVD).Atmospheric Pressure Chemical Vapor Deposition (APCVD).Other types of CVD (LPCVD, PECVD, HDPCVD…).Introduction to evaporation.Evaporation tools and issues, shadow evaporation.Introduction to sputtering and DC plasma.Sputtering yield, step coverage, film morphology.Sputter deposition: reactive, RF, bias, magnetron, collimated, and ion beam.Deposition methods for thin films in IC fabrication.Atomic layer deposition (ALD).Pulsed laser deposition (PLD).Epitaxy (CVD or vapor phase epitaxy , molecular beam epitaxy).NE 343: Microfabrication and thin film technologyInstructor: Bo Cui, ECE, University of Waterloo;Textbook: Silicon VLSI Technology by Plummer, Deal and Griffin
2 Common deposition methods for thin films in IC fabrication
3 Epitaxial silicon deposition Advantages of epitaxial wafers over bulk wafersOffers means of controlling the doping profile (e.g. lightly doped on heavily doped possible)Epitaxial layers are generally oxygen and carbon freeGases used iin siilliicon epiittaxy
4 Chemical reactionsConcentration o of species at different positions along a horizontal reactor (carrier gas should be H2)SiCl4 + 2H2 Si + 4HClSiCl4 concentration decreases while the other three constituents (SiHCl3, SiH2Cl2, HCl) increase.
5 Equipment Three basic reactor configurations Weight 2000 Kg Occupy 2m2 or more of floor space.Quartz reaction chamber with susceptorsGraphite susceptors for physical support.A coating of silicon carbide (50 to 500 μm) applied by CVD process on susceptors.RF heating coil or tungsten halogen lamps (cold wall), water cooling.
7 Si APCVD epitaxy growth process Hydrogen gas purges of air from the reactor.Reactor is heated to a temperature.After thermal equilibrium, an HCl etch takes place at 1150oC and 1200oC for 3 minutes.Temperature is reduced to growth temperature.Silicon source and dopant flows are turned on.After growth, temperature is reduced by shutting off power.Hydrogen flow replaced by nitrogen flow.Depending on wafer diameter and reactor type, 10 to 50 wafers per batch can be formed.Process cycle times are about one hour.Epitaxy film need high temperature (>1000oC) because at high temperature the (amorphous) native oxide will become unstable and desorb from the surface, exposing the single crystalline silicon lattice for epitaxy.
8 Arsine doping and growth processes 2AsH3 (gas) 2As (solid) + 3H2 (gas)Interaction between doping process & growth processGrowth rate influences the amount of dopant incorporated in SiEquilibrium established at low growth rates.There is also auto-doping, which can be minimized by:Fast growth to minimize out-diffusion.Low temperature deposition reduces boron auto-doping (not As however).Seal backside of substrate with highly doped poly-oxide.Avoid the use of HCl etching.Reduced pressure epitaxy.
9 Polycrystalline silicon deposition Application: gate of MOSFET.Usually deposited in a LPCVD chamber at Pa, oC, 10-20nm/min.SiH4 is preferred because of its lower deposition temperature.H2 carrier gas for solid curvesFigure 9-8Usually amorphous when deposition at <575oC; but may be polycrystalline if deposition rate is low enough.Columnar grain structure/texture, and the grain will grow when annealed.When annealed, amorphous Si will become polycrystalline Si with even large grain size than poly-Si under same annealing.1Torr = 132 Pa
10 Grain structure and resistivity Traps states (dopant inactive when trapped there) and scattering at grain boundary limits the resistivity.At higher doping, trap states are all filled and cannot further reduce active dopant concentration.
11 Deposition rate and oxidation of poly-Si Deposition rate should be pressure since rate ksCG/N for hG>>ks, but actually sub-linear.This is because at higher rate, it is determined by desorption of reaction product H2 (rather than gas transport onto the surface).Oxidation of poly-silicon:Usually oC dry oxidation.Un-doped or lightly doped poly-Si oxidizes at rate between that of (111) and (100) single crystal Si.P-doped poly-Si oxidizes faster than un-doped or lightly doped one.
12 Silicon nitride deposition Application:Masks to prevent oxidation for LOCOS processFinal passivation barrier for moisture and sodium contaminationEtch stop for Cu damascene processPopular membrane material by Si backside through-wafer wet etch.PECVDLPCVDCan also deposit nitride using silane at oC by APCVD; or use N2 gas instead of NH3.LPCVD conformal Si3N4 filmsLow-stress nitride deposition using DCS (dichloro-silane SiCl2H2)
13 Silicon nitride properties tensile orcompressiveLPCVD film quality is much better than PECVD in almost every aspect.
14 Silicon dioxide deposition Sputtered oxide has poorer step coverage than CVD.APCVD has been used for many years, but today LPCVD and PECVD are more popular.Silane based LPCVDTEOS (tetra-ethoxy-silane). LPCVD °C, PECVD 350°C. Lower sticking coefficient, thus more conformal film.Silane based PECVDOthersSiCl2H2 + 2N2O SiO2 + 2N2 + 2HCl (etches Si), 900oC, film contain Cl.TEOS + Ozone (O3). Ozone is more reactive and lowers deposition temperature to 400oC.
16 Improve step coverage by PSG reflow No P2.2% P4.6% P7.6% PAdd PH3 to source gas to get P- doped oxide: PSG - phosphosilicate glassPSG is more flow-able than oxide: reflow at oC to improve step coverage.Usually 6-8 wt% of P.Add B can further reduce reflow temperature (BPSG: borophosphosilicate glass)
18 Chapter 9 Thin film deposition Introduction to thin film deposition.Introduction to chemical vapor deposition (CVD).Atmospheric Pressure Chemical Vapor Deposition (APCVD).Other types of CVD (LPCVD, PECVD, HDPCVD…).Introduction to evaporation.Evaporation tools and issues, shadow evaporation.Introduction to sputtering and DC plasma.Sputtering yield, step coverage, film morphology.Sputter deposition: reactive, RF, bias, magnetron, collimated, and ion beam.Deposition methods for thin films in IC fabrication.Atomic layer deposition (ALD).Pulsed laser deposition (PLD).Epitaxy (CVD or vapor phase epitaxy , molecular beam epitaxy).NE 343: Microfabrication and Thin Film TechnologyInstructor: Bo Cui, ECE, University of Waterloo,Textbook: Silicon VLSI Technology by Plummer, Deal, Griffin
19 Atomic layer deposition (ALD, break CVD into two steps) Similar in chemistry to CVD, except that the ALD reaction breaks the CVD reaction into two half-reactions, keeping the precursor materials separate during the reaction.The precursor gas is introduced into the process chamber and produces a monolayer of gas on the wafer surface. A second precursor gas is then introduced into the chamber reacting with the first precursor to produce a monolayer of film on the wafer surface.Film growth is self-limited (monolayer adsorption/reaction each half-cycle), hence atomic layer thickness control of film growth can be obtained.That is, one layer per cycle; thus the resulting film thickness may be precisely controlled by the number of deposition cycles.Two fundamental mechanisms:Chemi-sorption saturation processSequential surface chemical reaction processIntroduced in 1974 by Dr. Tuomo Suntola and co-workers in Finland to improve the quality of ZnS films used in electroluminescent displays.Recently, it turned out that ALD also produces outstanding dielectric layers and attracts semiconductor industries for making High-K dielectric materials.
20 Example: ALD cycle for Al2O3 deposition 1. Introduce TMA(tri-methyl aluminum)In air, H2O vapor absorb on Si to form Si-O-H.2. TMA reacts with hydroxyl groups to produce methane.
21 ALD cycle for Al2O3 deposition 3. Introduce H2O. Reaction product methane is pumped away, leaving an OH- passivation layer on surface.4. After three cycles.One TMA and one H2O vapor pulse form one cycle. Here 1Å/cycle, each cycle including gas injection and pumping takes few seconds.Two steps each cycle
22 Closed system chambers (most common) for ALD The reaction chamber walls are designed to effect the transport of the precursors.
23 Advantages and disadvantages ALD: slowest, best step coverageAdvantagesStoichiometric films with large area uniformity and 3D conformality.Precise thickness control.Low temperature deposition possible.Gentle deposition process for sensitive substrates.DisadvantagesDeposition rate slower than CVD.Number of different materials that can be deposited is fair compared to MBE.
24 Chapter 9 Thin film deposition Introduction to thin film deposition.Introduction to chemical vapor deposition (CVD).Atmospheric Pressure Chemical Vapor Deposition (APCVD).Other types of CVD (LPCVD, PECVD, HDPCVD…).Introduction to evaporation.Evaporation tools and issues, shadow evaporation.Introduction to sputtering and DC plasma.Sputtering yield, step coverage, film morphology.Sputter deposition: reactive, RF, bias, magnetron, collimated, and ion beam.Deposition methods for thin films in IC fabrication.Atomic layer deposition (ALD).Pulsed laser deposition (PLD).Epitaxy (CVD or vapor phase epitaxy , molecular beam epitaxy).NE 343: Microfabrication and Thin Film TechnologyInstructor: Bo Cui, ECE, University of Waterloo,Textbook: Silicon VLSI Technology by Plummer, Deal, Griffin
25 Pulsed laser deposition (PLD) PLD Characteristics:Reproduce the composition of the targetFast response, well controlled deposition rateEnvironmentally benign techniqueFlexible, easy to implement.Growth in any environment.Atoms arrive in bunches.Uneven coverage.High defect or particulate concentration.Not well suited for large-scale film growth.Two targets, co-deposition
26 Plume generated by laser ablation with different tiny or micro-particles Pulse of fs to ns with peak power high enough (hundreds of MW/cm2) to melt → boil → vaporize → ablate the target surface material, to atoms, ions, electrons, and clusters.Laser BeamTargetSubstratePlume(plasma)(a)(b)(c)(d)Laser-material interaction. (a) Absorption and heating; (b) Melting and flowing; (c) Vaporization; (d) Plasma formation in front of the target. Under certain conditions the plasma can detach from the target and propagate toward the laser beam.Pulse duration < 10 psCollisional and multi-photon ionization.Plasma formation without melting.Deviation from 1/2 scaling.Pulse duration > 50 psConventional melting, boiling and fracture.Threshold fluence (J/cm2) for ablation scales as 1/2.
27 PLD physicsMetals, absorption depth 10 nm, depending on wavelength.Relaxation of energy 1 ps, electron-phonon interaction.Incredibly non-equilibrium!!At peak of laser pulse, temperature on target can reach >105 K (> 40 eV!)Electric field > 105 V/cm, also high magnetic fieldsPlasma temperature KAblated species with energy 1–100 eVIt is also an excellent micro-machining tool, with clean-cut profile.
28 Transient plume development 10-6Torr vacuum(plasma of vapor of target material)100 mTorr O2(plasma of O2 and vapor of target material)D. Geohegan, Appl. Phys. Lett. 60, 2732 (1992)
29 Pulsed laser deposition (PLD) system View WindowsExcimer laserChamberAnother system
31 (Mesoscopic Integrated Conformal Electronics) DARPA MICE program(Mesoscopic Integrated Conformal Electronics)Single (pulsed) laser does surface pretreatment, spatially selective material deposition, surface annealing, component trimming, ablative micromachining, dicing and via-drillingDirect writing of electronic components- in air!Rapid process refinementNo masks, pre-forms, or long cycle timesTrue 3-D structure fabrication possibleDARPA: Defense Advanced Research Projects Agency, major US funding agency
32 Chapter 9 Thin film deposition Introduction to thin film deposition.Introduction to chemical vapor deposition (CVD).Atmospheric Pressure Chemical Vapor Deposition (APCVD).Other types of CVD (LPCVD, PECVD, HDPCVD…).Introduction to evaporation.Evaporation tools and issues, shadow evaporation.Introduction to sputtering and DC plasma.Sputtering yield, step coverage, film morphology.Sputter deposition: reactive, RF, bias, magnetron, collimated, and ion beam.Deposition methods for thin films in IC fabrication.Atomic layer deposition (ALD).Pulsed laser deposition (PLD).Epitaxy (CVD or vapor phase epitaxy , molecular beam epitaxy).NE 343: Microfabrication and Thin Film TechnologyInstructor: Bo Cui, ECE, University of Waterloo,Textbook: Silicon VLSI Technology by Plummer, Deal, Griffin
33 IntroductionEpitaxy refers to the method of depositing a monocrystalline film on a monocrystalline substrate.The word “epitaxy” comes from the Greek for ‘above’ (epi) and ‘in an ordered manner’ (taxis): to arrange upon.Autoepitaxy(or Homoepitaxy): extension of the substrate lattice by the overgrowth of a layer of identical material (e.g. Si on Si or GaAs on GaAs) with no problem of compatibility or mismatch.Heteroepitaxy: any two materials of different crystalline structure and orientation (e.g. (001) GaAs on (001) Si or (001) Si on Sapphire)EpitaxyEpilayerInitial substrate33Most slides in this section prepared by Ehsan Fathi
34 Heteroepitaxy conditions Substrate must be physically and chemically inert to the growth environment and being prepared with a damage-free surface.Chemical compatibility between the materials to avoid compound formation or massive dissolution of one layer by the other.Matched thermal expansion characteristics between the layer and substrate to avoid excess stress upon cooling → formation of dislocation at the interface, or even breaking of the structureMatched lattice parameters between the layer and substrate → not a serious problem34
35 Strained and unstrained Schematic illustration of (a) lattice-matched, (b) strained, and (c) relaxed hetero-epitaxial structures. Homoepitaxy is structurally identical to the lattice-matched heteroepitaxy.35
36 Strained and unstrained Experimentally determined critical layer thickness for defect-free, strained-layer epitaxy of GexSi1-x on Si, and Ga1-xInxAs on GaAs.36
37 Strained-layer superlattices Strained-layer superlattices : in some devices we need repeated, regular alternation between two monocrystallineWith these structures we can alter the basic physical properties of the materialBecause the layers are sufficiently thin, the lattice mismatch is accommodated by uniform strains in the layers.The new lattice will have an equilibrium lattice constant b such that a1 > b > a2 (for a1 > a2)direction of the strain37
38 Growth methodsVapor-Phase Epitaxy (VPE, a form of CVD): transport of the epilayer constituents (Si, Ga, As, dopants,…) in the form of one or more volatile compounds to the substrate where they react to form the epilayer.Molecular Beam Epitaxy: physical transport of material to a heated substrate through vacuum evaporation.Liquid-Phase Epitaxy (LPE): the growth of epitaxial layer on crystalline substrate by direct precipitation from the liquid phase.38
39 Silicon VPESiCl4, SiH2Cl2, SiHCl3, and SiH4 have been used for VPE growth.Silicon tetrachloride is the most studied and has the widest industrial use.Other silicon sources are used because of lower reaction temperature.@ 1200 oCAn additional competing reaction is taking place:If the silicon tetrachloride concentration is too high, etching rather than growth of silicon will take place.If the carrier gas entering the reactor contains hydrochloric acid, etching will take place.This etching is used for in-situ cleaning of the Si wafer prior to epitaxial growth.39
40 The halide process for GaAs deposition In this process transport of gallium accomplished by means of the halide, AsCl3.Both hydrogen and AsCl3 vapor enter the system and they react:This reaction product flow over the gallium source and GaAs formed as a crust on the surface of galliumThe HCl gas resulting from the first reaction transfer gallium to the substrate in the form of GaCl, where the GaAs is 750 oC:Should be fully saturated with As40
41 The hydride process for GaAs deposition Fluxes of gallium and arsenic species formed independently → greater control in the vapor phase, and hence a wider control of the deposition parametersAs4 for As, and gallium chloride (GaCl) for Ga component are used.As4 is generated by thermal decomposition of arsine (AsH3):Gallium chloride is generated by the reaction:For In-situ etching41
42 The organometallic process MOCVD: metal-organic CVD = OMVPE: organo-metallic vapor phase epitaxyHalide and hydride processes cannot be extended to the growth of AlGaAs by the simultaneous growth of GaAs and AlAs ( growth of AlAs occurs ~ 1100oC).This problem avoided in the organometalic process.Many materials that we wish to deposit have very low vapor pressures and thus are difficult to transport via gases.One solution is to chemically attach the metal (Ga, Al, Cu, etc…) to an organic compound that has a very high vapor pressure.• The organic-metal bond is very weak and can be broken via thermal means on wafer, depositing the metal with the high vapor pressure organic being pumped away.Some MOCVD precursor gases:Tri-methyl-aluminum, liquidTri-methyl-gallium, liquidArsine AsH3, gasDi-methyl selenide, liquidDi-methyl zinc, liquid42
43 The organometallic process Advantages: Highly flexible → we can deposit semiconductors, metals, dielectricsDisadvantages: Highly toxic, very expensive source material, and environmental disposal costs are high.Material deposited:III-V semiconductors - AlGaAs, AlGaInP, AlGaN, AlGaP, GaAsP, GaAs, GaN, GaP, InAlAs, InAlP, InSb , InGaN, GaInAlAs, GaInAlN, GaInAsN, GaInAsP, GaInAs, GaInP, InN, InP.II-VI semiconductors - Zinc selenide (ZnSe), HgCdTe, ZnO, Zinc sulfide (ZnS)IV semiconductors - Si, Ge, strained silicon43
44 Molecular-beam epitaxy (MBE) MBE is an epitaxial process involving the reaction of one or more thermal beams of atoms or molecules with a crystalline surface under UHV conditions.Precise control in both chemical composition and doping profiles.It has a very low growth rate (e.g. for GaAs, a value of 1μm/hr is typical.)Single-crystal multilayer structures with dimensions on the order of atomic layers can be made.Diagnostic tools44
45 Effusion cell (Knudsen cell) The most common type of MBE source is the effusion cell. Sources of this type are sometimes called Knudsen, or K-cells.The crucible and source material are heated by radiation from a resistively heated filament. A thermocouple is used to allow closed-loop feedback control.A typical Knudsen cell contains a crucible (made of pyrolytic boron nitride (PBN), quartz, tungsten or graphite), heating filaments (often made of metal tantalum), water cooling system, heat shields and shutter.PBN crucibleResistive heater filament3. Metal foil radiation shields4. Thermocouple5. Mounting flange45
46 RHEEDReflection high-energy electron diffraction (RHEED) is a technique used to characterize the surface of crystalline materials.A RHEED system consist of an electron source (gun), and a photoluminescent detector screen.The electron gun generates a beam of electrons which strike the sample at a very small angle relative to the sample surface.Incident electrons diffract from atoms at the surface of the sample, interfere constructively at specific angles and form regular patterns.46
47 RHEEDThe 3D surface results in a spotty pattern due to the electron transmission through surface roughness.The more 2D surface giving rise to the commonly observed RHEED streaks.47
49 Liquid-phase epitaxy (LPE) LPE involves the growth of epitaxial layers on crystalline substrate by direct precipitation from the liquid phase.In LPE, the substrate is held in contact with the supersaturated solution (As saturated solution of Ga).Cooling the arsenic saturated solution of gallium causes the arsenic to precipitate in the form of GaAs.Typical deposition rates for monocrystalline films range from 0.1 to 1 μm/min.LPE in most cases is a very economic deposition techniques, especially when up-scaled to mass-production49
Your consent to our cookies if you continue to use this website.